BENDING STRENGTH, STIFFNESS, AND STRESS-GRADE OF STRUCTURAL PINUS RADIATA:
EFFECT OF KNOTS AND TIMBER DENSITY
D. J. GRANT, A. ANTON and P. LIND Forestry Commission of N.S.W., P.O. Box 100, Beecroft,
New South Wales 2119, Australia
(Received for publication 26 March 1984; revision 22 November 1984)
ABSTRACT Australian-grown Pinus radiata D. Don (radiata pine) timber of 35 x 70 mm,
35 x 90 mm, and 45 x 90 mm cross-section was mechanically graded and then tested in bending to determine modulus of elasticity (MOE) and modulus of rupture (MOR). Knots contributing to failure were measured and classified and their knot area ratio calculated. The air-dry density of the timber was also determined.
Accuracy of prediction of MOR using MOE was shown to be independent of timber density but was improved by including knot area ratio, and sometimes knot position, in the regression.
Reductions in timber density and increases in knot size reduce theoretical mechanical stress-grade yields. Therefore a reduction in the market value of sawn structural timber is predicted if forest management aims to increase the rate of growth of plantation trees without compensatory attention to density and branch size.
When the radiata pine timber used in the study was graded to the normal Australian visual grading rules, it generally failed to meet normal bending strength requirements. A re-assessment of the grading rules is recommended.
This study investigated the effect of knot size and timber density on bending strength, fiexural stiffness, and, by implication, stress-grade recoveries in radiata pine scantling.
The main aim of grading timber for strength is to prevent material of inferior quality entering any one specified stress-grade. A stress-grade is usually defined as:
"The classification of a piece of timber for structural purposes by means of either visual or mechanical grading to indicate primarily the basic working stress in bending for purposes of design and, by implication, the basic working stresses for other properties normally used in engineering design. The stress grade is designated in a form such as T7' which indicates that, for such a grade of material, the basic working stress in bending is approximately 7 MPa" (SAA 1975).
New Zealand Journal of Forestry Science 14(3): 331-48 (1984)
332 New Zealand Journal of Forestry Science 14(3)
Hence bending strength is of primary importance in the determination of a stress-grade. In general, the visual and mechanical grading systems use one or more measur-able parameters to assign a stress-grade to timber, the primary parameters being knots in visual grading and flexural stiffness in mechanical grading.
Mechanical grading consists of three distinct steps. Firstly, timber stiffness is measured in a machine that sprays a colour on to the timber to indicate a stiffness range; secondly, a visual inspection is carried out for the detection of defects likely to reduce the shear strength or utility of the piece, or for excessive defects in the un-measured section; and thirdly, a grade stamp is applied.
Visual grading "is accomplished from an examination of all four faces and the ends of the piece, in which the location as well as the size and nature of the knots and other features appearing on the surfaces are evaluated over the entire length" (ASTM 1974).
Mechanical grading uses measured stiffness as an indicator for strength and utilises the correlation that exists between short-span apparent modulus of elasticity (MOE) measured on the flat and modulus of rupture (MOR) measured on edge in order to predict strength. Mechanical grading programs are determined by the testing of full-sized sections of timber, followed by analysis of MOR results for specimens within various MOE ranges and then the assignment of a stress-grade (F grade) to timber within those MOE ranges (Anton 1977, 1981).
Until very recently, visual grading rules have been based entirely on the methods of ASTM D245-74, "Establishing Structural Grades and Related Allowable Properties for Visually Graded Lumber (ASTM 1974) -
"The development of these methods was based on extensive research in the United States covering tests of small clear specimens and of full-sized structural members. Detailed studies included the strength and variability of clear wood, and the effect on strength from various factors such as density, knots and other defects, seasoning, duration of stress, and temperature."
Direct application of these visual grading methods, however, without adequate verifica-tion of their accuracy by the testing of full-sized, graded, specimens has been under question for some years. Effects of density and, in particular, knot type and size on the strength of full-sized specimens are therefore of significance in the resolution of these arguments, at least for radiata pine.
MATERIALS AND METHODS Approximately 300 mechanical stress-grading quality assurance test specimens
(SAA 1978) of 35 X 90 mm cross-section were used initially to develop a standard method of notation and measurement. These specimens were routine samples from sawmills in New South Wales (Tumut and Bathurst), Australian Capital Territory, Victoria (Myrtleford), South Australia (Mount Gambier), and Tasmania (Scottsdale). A further 1200 pieces of 35 X 70 mm and 45 X 90 mm were obtained from grading operations in Bathurst, Myrtleford, Scottsdale, and Mt Gambier, with approximately equal representation from each State.
The Australian Standard for visually stress-graded radiata pine (SAA 1973) describes
Grant et al. Bending strength, stiffness, and stress-grade 333
most of the defects likely to be present in radiata pine scantling and was used as a basis for knot description. Recording of defect size and position was straightforward except where a combination of defects occurred and particularly when they were of differing types. In these specimens the size and position of the defect that contributed to the failure were determined after fracture. If more than one defect contributed to failure and the combination was not implicitly covered by the Australian Standard then the knot sizes were left unrecorded. It was not possible to describe some defects and they also were not recorded. Specimens that contained any growth rings with a diameter of less than 50 mm were excluded in line with the visual grading rules for radiata pine (SAA 1973).
Apparent MOE and MOR were determined in accordance with AS 1749, Appendix A (SAA 1978). MOE was determined with the specimen loaded at mid-span simply supported as a plank over a 914-mm span with the defective section in the middle. MOR was determined with the specimen loaded as a joist in four-point bending with the subjectively worst strength-reducing defect on the tension side. Span to depth ratio was about 14 to 1. After failure each specimen was checked against the recorded defect type to ensure the defect contributing to failure had been correctly recorded.
Density was determined for the 35 X 70-mm and 45 X 90-mm sizes by weighing the 1.5-m long specimens after they had been conditioned to approximately 12% moisture content. The density of the 35 X 90-mm specimens was determined from a section 140 X 22 X 22 mm in cross-section taken from each specimen for the evaluation of some clear timber properties as part of a separate project. These were also conditioned to approximately 12% moisture content.
Knot area was calculated using the normally accepted method of projecting the knot on to a cross-sectional plane. Knot area ratio (KAR) was calculated by dividing the total knot area by the cross-sectional area of the specimen.
RESULTS AND DISCUSSION Knot types that were sufficiently well represented to permit separate analysis were
margin, face, arris, and a special type of margin knot called margin/face (Fig. 1). Approximately 800 fell into this category and, as a grouping, it would represent around 70% of the defects in heart-excluded radiata pine scantling generally.
Margin Face Margin/Face 3
Arris FIG. 1Cross-sectional representation of the knot types included in the study.
334 New Zealand Journal of Forestry Science 14(3)
Group univariate statistics of MOE, MOR, density, and KAR are given in Tables 1 to 4. Mean MOR (Table 2) was generally independent of cross-section except for the 55 X 70-mm and 45 X 90-mm margin/face knot groups, the 35 X 70-mm and 45 X 90-mm arris knot groups, and the 35 X 90-mm and 45 X 90-mm arris knot groups. Both the margin and margin/face knots had a similar, lower, mean strength than the face and arris knots because of a larger percentage of knots in the highest stressed area of the timber during testing.
There was no significant difference at the 1% level between mean density for any of the 12 groups (Table 3) indicating that timber density was independent of both cross-section and knot type groupings.
TABLE 1Modulus of elasticity statistics for all groups (GPa)
35 X 70 35 X 90 45 X 90
35 X 70 35 X 90 45 X 90
35 X 70 35 X 90 45 X 90
35 X 70 35 X 90 45 X 90
79 47 46
31 41 48
9.08 9.32 8.89
8.82 9.13 8.90
8.33 8.69 8.19
2.48 2.58 2.12
2.34 2.63 2.51
2.06 2.59 2.10
2.58 2.44 2.21
3.80 4.82 4.94
3.77 4.30 4.76
4.53 4.13 4.05
3.79 4.74 5.08
15.69 16.23 13.87
13.96 14.99 14.48
12.98 16.25 13.94